Synthesis of zigzag- and fjord-edged nanographene with dual amplified spontaneous emission

We report the synthesis of a dibenzodinaphthocoronene (DBDNC) derivative as a novel nanographene with armchair, zigzag, and fjord edges, which was characterized by NMR and X-ray crystallography as well as infrared (IR) and Raman spectroscopies. Ultrafast transient absorption (TA) spectroscopy revealed the presence of stimulated emission signals at 655 nm and 710 nm with a relatively long lifetime, which resulted in dual amplified spontaneous emission (ASE) bands under ns-pulsed excitation, indicating the promise of DBNDC as a near-infrared (NIR) fluorophore for photonics. Our results provide new insight into the design of nanographene with intriguing optical properties by incorporating fjord edges.

In contrast to the planar armchair and zigzag edges, cove and ord edges, corresponding to [4] and [5] helicenes, respectively, enforce twisted congurations, providing direct access to nonplanar NGs. 5,31 While a number of cove-or ordedged NGs with unique contorted and/or twisted conformations and intriguing (opto)electronic and supramolecular properties have been reported, 31-33 their combination with extended zigzag edges (three or more benzene rings) has remained rare. Helianthrene, originally reported by H. Brockmann in 1942 (Fig. 1), 34 can be considered a classical example of this category, which was known for its high reactivity with oxygen to form the endoperoxide. [35][36][37][38][39][40][41] Bistetracene with a combination of zigzag and ord edges was more recently synthesized to show an open-shell character. 42 Although the initially reported bistetracene derivative was unstable and oxidized under ambient conditions, kinetic protection with four substituents on the zigzag edges allowed for the stabilization and integration into eld-effect transistor devices, demonstrating promising bipolar charge transport properties. 43 Herein, we report the synthesis and characterization of dibenzo[a,m]dinaphtho [3,2,1-ef:1 ′ ,2 ′ ,3 ′ -hi]coronene (DBDNC) 1 as a novel NG with ord and extended zigzag edges, which demonstrated high stability and strong red emission. The nonplanar structure of DBDNC 1 was unambiguously revealed by X-ray crystallography, and its vibrational properties were investigated by infrared (IR) and Raman spectroscopies supported by density functional theory (DFT) calculations. Moreover, the in-depth investigations of the photophysical properties of 1 by ultrafast transient absorption (TA) spectroscopy and photoluminescence spectroscopy under ns-pulsed excitation revealed the occurrence of long-lived near-infrared (NIR) stimulated emission transitions as well as dual amplied spontaneous emission.
When the reaction time was extended to 4 h, a signal at m/z = 920.6 was observed, suggesting the formation of one additional C-C bond, presumably at the ord region, leading to 10,17-ditert-butyl-7,20-dimesityltetrabenzo [a,g,mn,pq]ovalene (TBOV) (Fig. S21 †). However, this product could not be isolated due to its low stability, being prone to oxidation (Fig. S22 †), precluding the structural characterization. Well-resolved 1 H and 13 C NMR spectra of DBDNC 1 could be recorded in a mixture of tetrahydrofuran (THF) and carbon disulde (CS 2 ), and the aromatic proton signals could be assigned with 1 H-1 H correlation spectroscopy (COSY) measurements ( Fig. 2 and S17-S19 †).
The single crystal of DBDNC 1 was obtained through evaporation of its solution in benzene/methanol, enabling structural analysis by X-ray crystallography. The structure of DBDNC 1 with the nonplanarity induced by the ord edge was thus clearly demonstrated. The vertical distance of ord-edged periphery between the centroids of rings A and A ′ is in the range of 2.345 A, resulting in a torsion angle of ∼49.5° (Fig. 3a, b and S23c †). The two mesityl groups are tilted with dihedral angles of 82°-83°. In the packing structure of DBDNC 1, there are two pairs of enantiomers with a racemate of (P)-1 and (M)-1 in the unit cell ( Fig. S23b †). No obvious intermolecular p-p interaction was observed apparently due to the existence of nonplanar ord edges as well as the tert-butyl and mesityl groups at the peripheral positions. To investigate the aromaticity of DBDNC 1, nucleus-independent chemical shis (NICS) 45 were calculated at GIAO-B3LYP/6-31G(d,p) level of theory. As shown in Fig. 3a, rings A, A ′ , B, and B ′ displayed large negative NICS(1) zz values (red color), indicating strong aromaticity at the ord region. The NICS(1) zz values of rings D, D ′ and H are 3.82, 2.94, and 1.45 (blue color), respectively, which suggests non-aromatic characters. This result agreed with an anisotropies of the induced current density (ACID) 46,47 plot calculated for non-substituted DBDNC, only including the p-electrons, which showed interruption of the diatropic ring currents at the D, D ′ and H rings (Fig. S25 †).
The IR and Raman spectra were recorded on a powder sample of DBDNC 1 and compared with the DFT-simulated spectra, displaying good agreement (Fig. 3). The out-of-plane CH bending region of the IR spectrum of DBDNC 1 showed  signicant vibrational ngerprints that can be associated with the molecular structure through the topology of the CH groups placed at the edge of the aromatic moieties, classied as SOLO, DUO, and QUATRO ( Fig. 3c; see the ESI † for details). 48 Briey, the strong IR peak at 757 cm −1 (762 cm −1 , scaled, DFT) could be assigned to the QUATRO mode, corresponding to the ord edge. The DUO and SOLO modes from the armchair and zigzag edges were found at 811 and 873 cm −1 (815 and 862 cm −1 , scaled, DFT), respectively. Moreover, other calculated IR-active normal modes of DBDNC 1 were also carefully inspected to obtain the band assignments summarized in Table S3, † with the graphical representation of the most IR-active modes in Table S4. † The measured and calculated Raman spectra of DBDNC 1 show a D band at approximately 1300 cm −1 and a G band near 1600 cm −1 (Fig. 3d), which account for ring-breathing and ring-stretching modes, respectively, in the aromatic core of DBDNC 1 (Fig. S27 †). The assignment of the representative Raman-active vibrational normal modes of DBDNC 1 are summarized in Tables S5 and S6. † The electrochemical properties of DBDNC 1 were investigated by cyclic voltammetry (CV) in dichloromethane with ferrocene as an external standard (Fig. S28 †). We observed two reversible oxidation peaks and one reversible reduction, with half-wave potentials respectively at E 1/2ox = +0.05 V and +0.61 V and at E 1/2red = −1.69 V with reference to Fc/Fc + . The HOMO and LUMO energy levels were estimated to be −4.85 eV and −3.17 eV based on the onsets of the oxidation and reduction peaks, respectively. Thus, the electrochemical energy gap was determined to be 1.68 eV.
The UV/vis absorption spectrum of DBDNC 1 in toluene was clearly structured with maxima at 633, 582, and 373 nm  Selected peaks are labeled with their wavenumbers (cm −1 ). The wavenumbers computed by DFT were uniformly scaled by 0.98. (Fig. 4a), which agreed with simulation by TD-DFT calculations at the CAM-B3LYP/6-311G(d,p) level (Fig. S24 †). The longwavelength absorption maximum at 633 nm was assigned to the HOMO / LUMO transition calculated at 597 nm (f = 0.6769) (Fig. 4b and Table S1 †). Notably, the solution of DBDNC 1 in toluene showed negligible changes in the UV/vis spectrum over half a month at room temperature in ambient conditions (Fig. S29 †), indicating its high stability. The emission spectrum of DBDNC 1 in toluene displayed well-dened peaks at 643, 698, and 772 nm, which were assigned to the 0-0, 0-1, and 0-2 vibronic bands, respectively. The optical energy gap was estimated from the interface of the absorption and emission spectra to be ∼1.94 eV. The Stokes shi was as small as 10 nm (246 cm −1 ), which is a clear signature of the rigid structure of this nanographene molecule notwithstanding the ord edge. The absolute photoluminescence quantum yield (PLQY; F) was 53%, and the uorescence lifetime (s s ) was determined to be 8.5 ns (Fig. S30 †). According to the equations F = k r × s s and k r + k nr = s s −1 , the radiative (k r ) and nonradiative (k nr ) decay rate constants from the singlet excited state were determined to be 6.2 × 10 7 s −1 and 5.5 × 10 7 s −1 , respectively.
We employed TA spectroscopy to gain further insights into the photophysics of DBDNC 1. Specically, we observe a transient spectrum that includes an excited state absorption (ESA) in the visible range (ESA 1, 430-560 nm), a photobleaching (PB) signal convoluted with stimulated emission (SE, 0 ′ / 0) at 640 nm, a positive peak corresponding to SE (0 ′ / 1) at 710 nm, and another ESA in the NIR range at 730-800 nm (ESA 2) ( Fig. 4c and d shows the spectra and the associated time-decays, respectively). Although the spectral features resemble those of NGs with zigzag edges, including DBOV derivatives, 3,26,29 DBDNC 1 exhibits distinct features, especially in terms of SE. First, this signal is appreciably redshied toward the NIR region (i.e., 660 nm vs. 710 nm in DBOV-Mes-C12 (ref. 25 ) and DBDNC 1, respectively, Fig. 4e). This effect can be attributed to the relatively small optical gap (1.94 eV) of DBDNC 1. Furthermore, we note that the SE lifetime is appreciably longer in DBDNC 1 than in DBOV-Mes-C12 (Fig. 4f), although the signal of the former would be affected more by the energy gap law than the latter, owing to the longer SE wavelength. 49 In particular, for DBDNC 1 the SE relaxation can be modelled via two-exponentials (3 ps and 6 ns, due to internal conversion and radiative relaxation from the rst excited singlet S 1 ), while in DBOV-Mes-C12 we have an additional tting component (170 ps) that can be attributed to the absorption losses due to charge absorption in aggregates. 30 In addition, the relaxation from S 1 is sensibly longer in DBDNC 1 than in DBOV-Mes-C12 (i.e., 6 ns vs. 2 ns) likely owing to the enhanced electron delocalization in the former, which usually leads to an increase of the emission lifetime in NGs. 50 Remarkably, polystyrene (PS) thin lms doped with 1 wt% of DBDNC 1 demonstrated dual amplied spontaneous emission (ASE) under ns-pulsed excitation at 355 nm (Fig. 5a). The presence of ASE is a clear signature of optical amplication, which can be identied by the collapse of the broad PL spectrum into a narrow peak accompanied by the sudden increase of the output intensity (I out ) upon increasing the pump uence. Two different narrow ASE bands are observed at 655 and 700 nm with different threshold (E th ) values of 13 and 5.3 mJ cm −2 , respectively (Fig. 5b). These threshold values are high compared with state-of-the-art NGs used for lasing (30-300 mJ cm −2 ), 26,28,51 which present a single ASE band matching their second vibronic. Nevertheless, dual-ASE in NGs has rarely been reported, with FZ3 (ref. 50) and PP-Ar 52 being the only two known reported examples, to the best of our knowledge.
The ASE performance of 1 is comparable to that of these two NGs (see Table S8 †) and might be attributed to the existence of two vibronic progressions associated to different vibrational modes. The rst ASE peak might correspond to a low frequency bending mode (∼240 cm −1 ) that overlaps with the rst vibronic. Meanwhile, the second ASE peak might correspond to a collective aromatic CC stretching mode (∼1290 cm −1 ). These frequencies have been estimated from the energy difference between the rst PL vibronic (643 nm) and each ASE peak (655 and 700 nm). Additionally, the ESA band overlapped with SE at 710 nm plays an important role. Typically, SE can be found at both vibronic progressions, but reabsorption is much higher for the peak at 655 nm that is closer to the ground-state absorption band. Then, ASE is observed only from the peak associated to the CC stretching mode (700 nm) because there is a large difference between both thresholds. However, in the case of DBDNC 1, the detrimental effect of the ESA band introduces extra losses that compensate the threshold difference and both ASE bands become active. Besides, ground-state absorption remains still higher than ESA, which accounts for the threshold difference between both ASE bands. These detrimental effects associated to reabsorption and ESA certainly account for the higher thresholds of DBDNC 1 compared with state-of-the-art NGs, in which ASE is observed only from the second vibronic associated to the aromatic CC stretching mode with only a little or negligible presence of reabsorption and/or ESA.
Finally, the ASE photostability under ns-pulsed excitation was studied by pumping the lms uninterruptedly at the same position with a pump uence twice the ASE threshold (Table S8 and Fig. S32 †). The photostability half-life parameter is used to quantify the performance, which is dened as the time or number of pulses needed for the output intensity to become half its initial value. The PS lms doped with DBDNC 1 show lower photostability (t 1/2 = 400 pump pulses [40 s]) than other NGs with similar ASE performance (t 1/2 ∼ 10 5 pump pulses for FZ3 and PP-Ar). 49,51 Such difference might be due to a higher reactivity toward oxygen, considering the helianthrene substructure, or higher intersystem crossing rate associated to the ord edge.

Conclusions
In summary, we have achieved the synthesis of DBDNC 1 as a novel NG with ord and extended zigzag edges and a rare pextended analog of helianthrene. The nonplanar structure of DBDNC 1 was unambiguously elucidated by X-ray crystallography, and further conrmed by IR and Raman spectroscopies supported by DFT calculations, which also revealed the intriguing vibrational ngerprints precisely assignable, e.g., to ord, zigzag, and armchair edges. DBDNC 1 displayed a narrow optical energy gap (∼1.94 eV) and strong emission with the PLQY of 54%. Moreover, DBDNC 1 demonstrated NIR SE with a relatively long lifetime, which was not affected by the intermolecular charge transfer, in contrast to the planar DBOV-Mes-C12. Remarkably, PS thin lms doped with DBDNC 1 exhibited dual ASE at 655 and 700 nm under ns-pulsed excitation, showing its potential for applications in NIR photonics. This work also offers new insight for the design of a further variety of non-planar NGs with zigzag and ord edges with intriguing photophysical properties.

Data availability
Crystallographic data for DBDNC 1 has been deposited at the Cambridge Crystallographic Data Centre (CCDC number: 2167126) and can be obtained from www.ccdc.cam.ac.uk/ structures. Other data that support the ndings of this study are available within the manuscript and in the ESI † or from the corresponding authors upon reasonable request.

Conflicts of interest
There are no conicts to declare.